OPEN

received: 11 March 2016 accepted: 27 June 2016 Published: 15 July 2016

Theory of Multifarious Quantum Phases and Large Anomalous Hall Effect in Pyrochlore Iridate Thin Films Kyusung Hwang1 & Yong Baek Kim1,2,3 We theoretically investigate emergent quantum phases in the thin film geometries of the pyrochore iridates, where a number of exotic quantum ground states are proposed to occur in bulk materials as a result of the interplay between electron correlation and strong spin-orbit coupling. The fate of these bulk phases as well as novel quantum states that may arise only in the thin film platforms, are studied via a theoretical model that allows layer-dependent magnetic structures. It is found that the magnetic order develop in inhomogeneous fashions in the thin film geometries. This leads to a variety of magnetic metal phases with modulated magnetic ordering patterns across different layers. Both the bulk and boundary electronic states in these phases conspire to promote unusual electronic properties. In particular, such phases are akin to the Weyl semimetal phase in the bulk system and they would exhibit an unusually large anomalous Hall effect. As a new venue for emergent quantum phases, correlated electron systems with strong spin-orbit coupling have provided exciting playgrounds for quantum materials physics1–3. Pyrochlore iridates, R2Ir2O7 (R is a rare earth element or Y), are prominent examples of such systems and have been extensively studied in the last few years4–41. Various novel phases have been proposed to occur as the results of the interplay between electron correlation and strong spin-orbit coupling, which include Weyl semimetal4,5, topological insulator5,6, Chern insulator6,7, chiral spin liquid8, axion insulator4,9, non-fermi-liquid10, and topological Mott insulator11. A great deal of experimental effort has been put forward to realize such phases in a number of pyrochlore iridate systems12–33. Previous theoretical studies have shown that the emergence of many novel phases can be understood by starting from a quadratic band touching (QBT) semimetal in the paramagnetic state, where two doubly-degenerate bands touch quadratically at the zone center34. Upon increasing the interaction or the Hubbard U, the system develops the all-in/all-out (AIAO) magnetic order, which breaks the time reversal symmetry, but not the cubic symmetry of the lattice4,5,9,35. This results in the splitting of the previously doubly-degenerate bands. Then the crossing of two non-degenerate bands leads to the Weyl semimetal (WSM) phase, where a pair of Weyl fermions and their cubic symmetry equivalents appear4,5,9,35. Further increasing the interaction makes a pair of Weyl fermions to move into high symmetric points in the Brillouin zone and when they meet, a band gap opens up at the high symmetry points, leading to a fully gapped magnetic insulator. Most of the pyrochlore iridates show a finite temperature (semi)metal-insulator transition and develop a magnetic order in the low temperature insulating phase while Pr2Ir2O7 is the only member of the family, that remains paramagnetic down to a few Kelvin12,13,16. Various experiments on R = Eu, Y, Nd compounds show evidences for the AIAO magnetic order18,20,26. Remarkably, a recent angle-resolved photo-emission spectroscopy (ARPES) measurement shows that the paramagnetic state of Pr2Ir2O7 has the QBT at the zone center, confirming the basic theoretical picture30. On the other hand, a clear evidence for the Weyl semimetal phase in this class of materials is currently lacking. From the theoretical point of view, the region in the bulk phase diagram where the Weyl semimetal phase exists is

1

Department of Physics and Centre for Quantum Materials, University of Toronto, Toronto, Ontario M5S 1A7, Canada. 2Canadian Institute for Advanced Research/Quantum Materials Program, Toronto, Ontario M5G 1Z8, Canada. 3School of Physics, Korea Institute for Advanced Study, Seoul 130-722, Korea. Correspondence and requests for materials should be addressed to K.H. (email: [email protected]) or Y.B.K. (email: [email protected] utoronto.ca) Scientific Reports | 6:30017 | DOI: 10.1038/srep30017

1

www.nature.com/scientificreports/ limited to a narrow window of intermediate strength of the Hubbard U5,9,35, and it is perhaps difficult to identify such a phase in the bulk materials. In this work, we theoretically explore the emergence of novel magnetic metallic phases akin to the Weyl semimetal4,5,42, in thin film geometries of the pyrochlore iridates. The primary motivations for this study are twofold. First, one of the prominent signatures of the Weyl fermions in the bulk system is the presence of the Fermi arc at the surface4,5, which is rather difficult to study in the three-dimensional cubic crystal. In this thin film geometries, both of the surface and bulk states may be more easily probed at the same time. Secondly, another important signature of the Weyl fermions is the large anomalous Hall effect. When a pair of Weyl fermions are present, the Hall conductivity is of the order of e2/h or proportional to e2/h times the distance between two Weyl points in the Brillouin zone36. In the cubic crystal, there also exist other Weyl points related by the cubic symmetry, which leads to the cancellation of the Hall conductivity and zero anomalous Hall effect. Hence the broken cubic symmetry of the thin film geometries may resurrect the large anomalous Hall effect by nullifying the cancellation36. We consider various pyrochlore film geometries with the boundary surfaces along the [111] direction and a realistic film thickness. Employing the effective tight-binding model35 for the jeff = 1/2 states from Ir4+ ions on the thin film geometry, we explore topological and magnetic phases fostered by the interplay between electron correlation, boundary surfaces, and lowered symmetries. We choose a parameter regime where the corresponding bulk system exhibits (i) the semimetal with the QBT at the zone center in the paramagnetic state (ii) the Weyl semimetal at intermediate strength of the interaction, and (iii) a gapped magnetic insulator with the AIAO order in the large interaction limit. Both the layer-dependance of the magnetic order parameter and the corresponding electronic structure are investigated by performing the self-consistent unrestricted Hartree-Fock mean-field theory computations, where the magnetic moments in each layer are allowed to point in any direction. An important discovery in this work is the appearance of the modulated magnetic order in the thin film geometries, where the amplitude and canting angles of the magnetic moments change from one layer to the other. The magnetic order can be regarded as a canted version of the AIAO order with varied canting angles depending on the layers. As the interaction strength increases, the magnetic order develops at the boundary layers first and then spreads to the central parts of the film. In general, the magnetic orders at the boundary layers are stronger than those near the central layers in the weak to intermediate correlation regime. This means the effective electron correlation is bigger at the boundary compared to the ones near the central layers. For example, there is a regime where only the boundary layers are magnetically ordered and the central layers remain paramagnetic. This is an interesting situation where only thin film system may realize various different parts of the bulk phase diagram in different locations of the layers. Because of the modulated magnetic order, the resulting electronic structure reflects intricate combinations of the bulk (near the central layers) and boundary states. One of the most interesting phases in the thin film systems is the magnetic metal with the modulated magnetic order in the intermediate correlation regime, where the splitting of the QBT occurs via the inhomogeneous effective fields from different layers with varied strength of the magnetic order. Here a plethora of crossings of non-degenerate bands lead to a complex structure of the Berry flux with many “monopoles” and “anti-monopoles” in momentum space. These crossings represent the thin film version of the Weyl fermions and lead to a large anomalous Hall effect as the cubic symmetry is explicitly broken in the thin film geometries. We also demonstrate the appearance of a variety of inhomogeneous magnetic metal phases depending on the choice of the boundary layers. This raises the hope that one could control the nature of the bulk and surface states by making appropriate choices of the boundary lattices. It should be pointed out that the appearance of the modulated or inhomogeneous magnetic order is crucial for the Berry phase structure with many “monopoles” and “anti-monopoles”, and the resulting large anomalous Hall effect. In a previous study37 of the thin film geometries, the uniform magnetic order was assumed and the largest anomalous Hall effect was found to occur in the so-called “hidden topological phase”. Such a phase exists only for specific choices of boundary layers. As explained in detail in the main text, our study shows that the underlying physics is very different when the inhomogeneous magnetic order arises and the largest possible anomalous Hall effect can occur irrespective of the presence of such phases or different choices of boundary layers.

Results

A. Theoretical Model. We consider a generic model for the thin films of the pyrochlore iridates grown along the [111] direction, which has the structure of alternating kagome and triangular layers of Ir4+ ions. Such structures can be regarded as the stackings of the kagome-triangular-bilayers [Fig. 1(a,b)]. Only the lattice sites in a unit cell are shown in Fig. 1(b) for simplicity while the kagome and triangular layers are schematically represented by light blue and green sheets, respectively. In the thin film structures, there are three distinct choices for the top and bottom boundary surfaces: (i) kagome and kagome (KK) layers, (ii) triangular and triangular (TT) layers, and (iii) kagome and triangular (KT) layers. Regardless of the boundary choice, the [111] film geometry has the C3 rotation symmetry along the [111] axis. For the KK and TT boundary conditions, the system additionally has the inversion symmetry. To investigate electronic and magnetic structures allowed in the [111] pyrochlore films, we employ the following tight binding model (introduced in ref. 35) based on the jeff = 1/2 Kramers doublet43,44 of the Ir4+ itinerant electrons. H =

∑

(i , j ) ∈ NN

+

Scientific Reports | 6:30017 | DOI: 10.1038/srep30017

ci† (t1 2 + it 2d ij ⋅ σ) c j +

U ∑ni (ni − 1), 2 i

∑

(i , j ) ∈ NNN

(

)

ci† t1′ 2 + i t2′ Rij + t3′ Dij ⋅ σ c j (1)

2

www.nature.com/scientificreports/

Figure 1. Lattice structure of the Ir4+ ions in the [111] pyrochlore thin films. (a) Bilayer structure formed with the kagome (light blue) and triangular (green) layers of the Ir sites (balls). (b) Stacking of the bilayers. For simplicity, the figure only shows three bilayers and the sites in a corresponding unit cell. (c) The Brillouin zone of the pyrochlore film structures. Red arrows in (a) represent the lattice vectors in the film structures.

Figure 2. Phases of the theoretical model in Eq. (1). (a) Mean-field phase diagrams for the 3D bulk system and [111] thin films with twenty bilayers. The diagrams include the semimetal (SM; white), antiferromagnetic insulator (AFI; gray), Weyl semimetal (WSM; blue), and a variety of magnetic metal (MM; pink, cyan, green) phases. For the classification of the MM phases, see the main text. (b) AIAO magnetic ordering pattern in the AFI and MM phases. In the tetrahedron, the bottom three and top single sites belong to the kagome and triangular layers as labeled by K and T. The magnetic moments {〈Ji〉} (red arrows) point along the local axes (blue lines) with slight canting of the moments at the kagome sites.

where ci† = (ci†↑, ci†↓ ) and cj = (cj↑, cj↓)T are creation and annihilation operators for the jeff = 1/2 states with the pseudospin ↑, ↓. Here the jeff = 1/2 band is half-filled. The first two terms in the model Hamiltonian describe the symmetry-allowed electron hopping processes for the nearest-neighbours (NN) and next nearest-neighbours (NNN) with the spin-independent (t1, t1′), and spin-dependent hopping processes (t2, t2′, t3′). The two-by-two matrices, 2 and σ = (σx, σy, σz) are the identity and Pauli matrices. Readers interested in more details of the tight binding model including the 3D pseudo-vectors, dij, Rij, and Dij, are referred to ref. 35. The last term, expressed in terms of the electron density ni = ci† 2c i , represents the Hubbard on-site repulsion (U) to incorporate electron correlation. We choose the parameter regime: toxy = 1, tσ = −0.8, tπ = −2tσ/3, and tσ′/t σ = tπ′ /t π = 0.08 in the Slater-Koster parametrization for the hopping amplitudes of ref. 35. In the 3D bulk system with the same parameters, a mean-field theory leads to the SM with the QBT, WSM, and AFI with the AIAO order upon controlling U [see the 3D bulk phase diagram in Fig. 2(a)]. In this parameter regime, we construct a self-consistent mean-field theory for the [111] pyrochlore thin film with 20 bilayers for the three different boundary conditions: KK, TT, and KT. In this mean-field theory, the Hubbard 1 4 2 interaction term is decoupled via 2 ∑i ni (ni − 1) → − 3 Ji ⋅ Ji + 3 Ji 2 with Ji = 1 ci† σc i , and we allow 2 layer-dependent configurations 〈Ji〉 of the magnetic order. We solve the resulting mean-field Hamiltonian self-consistently for each boundary condition. The mean-field phase diagrams obtained for different boundary conditions are plotted in Fig. 2(a). We find three different classes of phases in the film systems: nonmagnetic semimetal (SM), antiferromagnetic insulator (AFI), and a variety of magnetic metal (MM) phases. In the subsequent sections, we explain the nature of these phases and describe their properties by focusing first on the results for the KK film shown in Figs 3 and 4. The cases for other boundary conditions (Figs 5–8) are then discussed in comparison with the KK film.

B. Magnetic Structure. We first describe the nature of different phases by investigating the magnetic properties. As in the 3D bulk system, the SM and AFI phases [white and grey in Fig. 2(a)] appear in the weak and strong correlation regimes, respectively, commonly for all three boundary conditions. A variety of magnetic

Scientific Reports | 6:30017 | DOI: 10.1038/srep30017

3

www.nature.com/scientificreports/

Figure 3. Magnetic structure of the KK film. (a) The local axis component 〈Ji〉l of the magnetic order parameter. The plot shows 〈Ji〉l as a function of U at the kagome boundary (KB; red) and central layer (C; orange) in the film. For comparison, the magnetic order parameter for the 3D bulk system (3D bulk; blue) is plotted together. (b) The electron density 〈ni〉with the same color scheme in (a). (c) Spatial profiles of 〈Ji〉l and 〈ni〉 over the layers (sublattices) in the KK film. (d) Spatial profiles of the canting component 〈Ji〉c of the magnetic order parameter for U = 1.50 (cyan), 1.52 (green), 2.00 (gray). (e) Sublattice index for the KK film with twenty bilayers. There are three sublattices on each kagome layer while only one on a triangular layer [see Fig. 1(b)].

Figure 4. Electronic structure of the KK film. (a) The Hall conductivity σxy as a function of U. (b) The magnetization M along the [111] direction as a function of U. (c) Electron band structures of the SM (U ≤ 1.30), MM-KB (U = 1.48, 1.50), and MM-C (U = 1.52) phases. In each plot, the surface modes localized at the top and bottom kagome layers (red and blue, respectively) are distinguished from the bulk bands (gray).

metallic (MM) phases appear in the intermediate correlation regime. Details of the magnetic structures in these phases are explained below. Semimetal. First, the nonmagnetic SM phase in the weak correlation regime is characterized by zero magnetic order parameter, 〈Ji〉 = 0. As will be discussed later, the electronic band structure of the SM can be regarded as the film version (finite size along the [111] direction) of the quadratic band touching at the Γpoint as seen in the corresponding 3D bulk phase. Scientific Reports | 6:30017 | DOI: 10.1038/srep30017

4

www.nature.com/scientificreports/

Figure 5. Magnetic structure of the TT film. (a) The local axis component 〈Ji〉l of the magnetic order parameter. The plot shows 〈Ji〉l as a function of U at the triangular boundary (TB; red) and central layer (C; orange) in the film. (b) The electron density 〈ni〉with the same color scheme in (a). (c) Spatial profiles of 〈Ji〉l and 〈ni〉over the layers (sublattices) in the TT film. (d) Spatial profiles of the canting component 〈Ji〉c of the magnetic order parameter for U = 1.30 (pink), 2.00 (gray). (e) Sublattice index for the TT film with twenty bilayers.

Antiferromagnetic insulator. The AFI phase in the strong correlation regime overall has the AIAO magnetic ordering pattern with slight modifications. The modifications occur in two different ways: (i) canting of the moments from the ideal AIAO ordering pattern, and (ii) layer-dependent modulation in the magnitude of the magnetic order parameter 〈Ji〉. The canting of the moments off the local axis arises on the kagome layers while the moments on the triangular layers are strictly along the local axis directions [Fig. 2(b)]. To characterize the canting of the moments, we decompose the magnetic order parameter 〈Ji〉into two parts: the component along the local axis (〈Ji〉l) and the perpendicular component representing the canting (〈Ji〉c). The left column of Fig. 3(c,d) show these components of the moments as functions of the sublattice index and U for the KK film. The sublattices are numbered sequently from the top to the bottom layers as shown in Fig. 3(e). Note that there are three sublattices on each kagome layer while only one on a triangular layer [Fig. 1(b)]. By comparing Fig. 3(c,d), we find that the canting component 〈Ji〉c is substantially small compared to the major component 〈Ji〉l along the local axis. In the case of U = 2 (gray), we clearly see the dominance of Ji l ( 0.40) over Ji c ( 0.06). As shown in the left column of Fig. 3(c), the size of the magnetic moment is modulated in different sublattices/layers. In general, magnetic order is stronger near the boundary layers rather than the central layers. This pattern is more evident in the MM phases [U = 1.34, 1.48, 1.50 in Fig. 3(c) left column] as explained further below. In spite of the canting of the moments and modulated magnetic order, it is found that the magnetic order in the film systems preserves the C3 rotation symmetry regardless of the boundary condition. In the KK and TT films, the inversion symmetry is also preserved in the presence of the magnetic order [Fig. 3(c,d)]. Magnetic metals. In the intermediate correlation regime, three distinct MM phases emerge as the electron correlation (U) increases in the film systems with various boundary conditions. The canting of the moments and the modulation of the magnetic order are more pronounced in this regime compared to the AFI phase in the strong correlation regime. Based on their magnetic structures at the boundary and central layers, we classify them into three different categories: (i) MM-TB, (ii) MM-KB, and (iii) MM-C. First, in the MM-TB and MM-KB phases, the magnetic order is present mainly around the boundary layers while the central layers are mostly non-magnetic. Here, the suffixes TB/KB mean that the triangular/kagome boundary layer has the magnetic order, respectively. In the MM-C phase, the magnetic order prevails in the central layers as well as near the boundaries. In general, the phases MM-TB, MM-KB, and MM-C appear sequently as the Hubbard U increases [see Fig. 2(a)]. More specifically, in the KK film, the MM-KB phase is found in the region 1.33